#------------------------------------------------------------------------------
#$Date: 2016-03-24 01:32:20 +0200 (Thu, 24 Mar 2016) $
#$Revision: 179534 $
#$URL: svn://www.crystallography.net/cod/cif/4/50/03/4500347.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4500347
loop_
_publ_author_name
'Nunes, Giovana G.'
'Seisenbaeva, Gulaim A.'
'Kessler, Vadim G.'
_publ_section_title
;
 Crystal Engineering of Nanomorphology for Complex Oxide Materials via
 Thermal Decomposition of Metal−Organic Frameworks. Case Study of
 Sodium Tantalate
;
_journal_issue                   4
_journal_name_full               'Crystal Growth & Design'
_journal_page_first              1238
_journal_paper_doi               10.1021/cg101456w
_journal_volume                  11
_journal_year                    2011
_chemical_formula_sum            'C30 H60 Na O12 Ta'
_chemical_formula_weight         816.72
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           12
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_atom_sites_solution_hydrogens   none
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.180(8)
_cell_angle_gamma                90.00
_cell_formula_units_Z            2
_cell_length_a                   17.394(12)
_cell_length_b                   10.049(7)
_cell_length_c                   8.404(6)
_cell_measurement_reflns_used    74
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      25.16
_cell_measurement_theta_min      3.61
_cell_volume                     1468.9(18)
_computing_cell_refinement       'Bruker Apex-II'
_computing_data_collection       'Bruker Apex-II'
_computing_data_reduction        'Bruker Apex-II'
_computing_molecular_graphics    'Bruker SHELXTL-NT'
_computing_publication_material  'Bruker SHELXTL-NT'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      296(2)
_diffrn_measured_fraction_theta_full 0.971
_diffrn_measured_fraction_theta_max 0.971
_diffrn_measurement_device_type  'Bruker SMART Apex-II'
_diffrn_measurement_method       'Omega Scan'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0210
_diffrn_reflns_av_sigmaI/netI    0.0184
_diffrn_reflns_limit_h_max       21
_diffrn_reflns_limit_h_min       -21
_diffrn_reflns_limit_k_max       11
_diffrn_reflns_limit_k_min       -12
_diffrn_reflns_limit_l_max       10
_diffrn_reflns_limit_l_min       -10
_diffrn_reflns_number            5818
_diffrn_reflns_theta_full        25.99
_diffrn_reflns_theta_max         25.99
_diffrn_reflns_theta_min         3.37
_exptl_absorpt_coefficient_mu    3.824
_exptl_absorpt_correction_T_max  0.7495
_exptl_absorpt_correction_T_min  0.3741
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'Bruker Apex-II'
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    1.847
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       prism
_exptl_crystal_F_000             840
_exptl_crystal_size_max          0.32
_exptl_crystal_size_mid          0.10
_exptl_crystal_size_min          0.08
_refine_diff_density_max         1.023
_refine_diff_density_min         -0.725
_refine_diff_density_rms         0.113
_refine_ls_extinction_coef       0.0064(14)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.372
_refine_ls_hydrogen_treatment    none
_refine_ls_matrix_type           full
_refine_ls_number_parameters     219
_refine_ls_number_reflns         1489
_refine_ls_number_restraints     377
_refine_ls_restrained_S_all      1.331
_refine_ls_R_factor_all          0.0312
_refine_ls_R_factor_gt           0.0306
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0499P)²+0.3082P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0767
_refine_ls_wR_factor_ref         0.0774
_reflns_number_gt                1475
_reflns_number_total             1489
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            cg101456w_si_001.cif
_cod_data_source_block           natapmc1
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Monoclinic' changed to 'monoclinic'
according to /home/saulius/struct/CIF-dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.1 from
2010-06-29.

'_exptl_absorpt_correction_type' value 'Multi-scan'
changed to 'multi-scan' according to
/home/saulius/struct/CIF-dictionaries/cif_core.dic dictionary named
'cif_core.dic' version 2.4.1 from 2010-06-29.

Automatic conversion script
Id: cif_fix_values 1715 2011-07-08 13:25:40Z adriana 

The following automatic conversions were performed:

'_exptl_crystal_density_meas' value 'not measured' was changed to '?'
- the value is perceived as not measured.

Automatic conversion script
Id: cif_fix_values 3008 2015-01-20 13:52:24Z robertas 
;
_cod_original_cell_volume        1468.9(17)
_cod_original_sg_symbol_H-M      C2/m
_cod_database_code               4500347
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, y, -z'
'x+1/2, y+1/2, z'
'-x+1/2, y+1/2, -z'
'-x, -y, -z'
'x, -y, z'
'-x+1/2, -y+1/2, -z'
'x+1/2, -y+1/2, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Ta1 Ta 0.0000 0.5000 0.5000 0.0423(2) Uani 1 4 d SU
O1 O -0.0894(7) 0.5412(14) 0.3666(17) 0.053(2) Uani 0.25 1 d PU
O2 O -0.0891(7) 0.5407(13) 0.6356(16) 0.049(2) Uani 0.25 1 d PU
O3 O -0.0647(9) 0.6126(18) 0.3650(17) 0.055(2) Uani 0.25 1 d PU
O4 O -0.0244(12) 0.6531(14) 0.3643(17) 0.054(2) Uani 0.25 1 d PU
O5 O -0.0649(9) 0.6134(16) 0.6365(15) 0.048(2) Uani 0.25 1 d PU
O6 O -0.0240(11) 0.6539(14) 0.6370(15) 0.049(2) Uani 0.25 1 d PU
C1 C -0.1411(5) 0.6413(11) 0.5923(11) 0.0514(15) Uani 0.50 1 d PU
C2 C -0.1412(5) 0.6420(11) 0.4077(11) 0.0524(16) Uani 0.50 1 d PU
C3 C 0.0004(6) 0.7826(9) 0.5922(10) 0.0481(17) Uani 0.50 1 d PU
C11 C -0.0967(8) 0.7873(12) 0.6467(15) 0.071(2) Uani 0.50 1 d PU
C12 C -0.0966(8) 0.7882(13) 0.3541(15) 0.073(2) Uani 0.50 1 d PU
C13 C -0.1927(9) 0.5000 0.646(2) 0.071(3) Uani 0.50 2 d SPU
C14 C -0.1918(9) 0.5000 0.353(2) 0.071(3) Uani 0.50 2 d SPU
C21 C -0.2196(13) 0.622(3) 0.332(3) 0.074(4) Uani 0.25 1 d PU
C22 C -0.2185(13) 0.622(3) 0.667(3) 0.071(4) Uani 0.25 1 d PU
C23 C -0.1704(14) 0.766(3) 0.668(3) 0.073(4) Uani 0.25 1 d PU
C24 C -0.0482(17) 0.889(2) 0.669(3) 0.071(5) Uani 0.25 1 d PU
C25 C -0.1699(15) 0.767(3) 0.331(3) 0.075(4) Uani 0.25 1 d PU
C26 C -0.0477(18) 0.890(2) 0.333(3) 0.073(5) Uani 0.25 1 d PU
Na1 Na -0.0001(4) 0.5000 0.1331(6) 0.0620(13) Uani 0.50 2 d SPU
O1A O -0.1116(10) 0.5000 -0.0001(17) 0.192(7) Uani 1 2 d SU
O2A O 0.0544(12) 0.3327(17) -0.001(2) 0.251(7) Uani 1 1 d U
C1A C 0.0372(19) 0.175(3) 0.005(5) 0.282(13) Uani 1 1 d U
C2A C -0.1865(16) 0.609(4) 0.000(4) 0.265(11) Uani 1 1 d U
C3A C -0.146(2) 0.725(5) 0.008(5) 0.300(13) Uani 1 1 d U
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ta Ta -0.7052 6.5227 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O3 Ta1 O3 180.0(8) 2_556 6_565
O3 Ta1 O3 70.7(12) 2_556 5_566
O3 Ta1 O3 109.3(12) 6_565 5_566
O3 Ta1 O3 109.3(12) 2_556 .
O3 Ta1 O3 70.7(12) 6_565 .
O3 Ta1 O3 180.000(2) 5_566 .
O3 Ta1 O1 24.7(6) 2_556 2_556
O3 Ta1 O1 155.3(6) 6_565 2_556
O3 Ta1 O1 48.4(8) 5_566 2_556
O3 Ta1 O1 131.6(8) . 2_556
O3 Ta1 O1 131.6(8) 2_556 .
O3 Ta1 O1 48.4(8) 6_565 .
O3 Ta1 O1 155.3(6) 5_566 .
O3 Ta1 O1 24.7(6) . .
O1 Ta1 O1 155.6(8) 2_556 .
O3 Ta1 O1 155.3(6) 2_556 6_565
O3 Ta1 O1 24.7(6) 6_565 6_565
O3 Ta1 O1 131.6(8) 5_566 6_565
O3 Ta1 O1 48.4(8) . 6_565
O1 Ta1 O1 180.000(1) 2_556 6_565
O1 Ta1 O1 24.4(8) . 6_565
O3 Ta1 O1 48.4(8) 2_556 5_566
O3 Ta1 O1 131.6(8) 6_565 5_566
O3 Ta1 O1 24.7(6) 5_566 5_566
O3 Ta1 O1 155.3(6) . 5_566
O1 Ta1 O1 24.4(8) 2_556 5_566
O1 Ta1 O1 180.000(2) . 5_566
O1 Ta1 O1 155.6(8) 6_565 5_566
O3 Ta1 O2 103.7(5) 2_556 6_565
O3 Ta1 O2 76.3(5) 6_565 6_565
O3 Ta1 O2 89.8(6) 5_566 6_565
O3 Ta1 O2 90.2(6) . 6_565
O1 Ta1 O2 109.7(6) 2_556 6_565
O1 Ta1 O2 75.5(6) . 6_565
O1 Ta1 O2 70.3(6) 6_565 6_565
O1 Ta1 O2 104.5(6) 5_566 6_565
O3 Ta1 O2 89.8(6) 2_556 .
O3 Ta1 O2 90.2(6) 6_565 .
O3 Ta1 O2 103.7(5) 5_566 .
O3 Ta1 O2 76.3(5) . .
O1 Ta1 O2 104.5(6) 2_556 .
O1 Ta1 O2 70.3(6) . .
O1 Ta1 O2 75.5(6) 6_565 .
O1 Ta1 O2 109.7(6) 5_566 .
O2 Ta1 O2 24.0(8) 6_565 .
O3 Ta1 O2 76.3(5) 2_556 2_556
O3 Ta1 O2 103.7(5) 6_565 2_556
O3 Ta1 O2 90.2(6) 5_566 2_556
O3 Ta1 O2 89.8(6) . 2_556
O1 Ta1 O2 70.3(6) 2_556 2_556
O1 Ta1 O2 104.5(6) . 2_556
O1 Ta1 O2 109.7(6) 6_565 2_556
O1 Ta1 O2 75.5(6) 5_566 2_556
O2 Ta1 O2 180.000(1) 6_565 2_556
O2 Ta1 O2 156.0(8) . 2_556
O3 Ta1 O2 90.2(6) 2_556 5_566
O3 Ta1 O2 89.8(6) 6_565 5_566
O3 Ta1 O2 76.3(5) 5_566 5_566
O3 Ta1 O2 103.7(5) . 5_566
O1 Ta1 O2 75.5(6) 2_556 5_566
O1 Ta1 O2 109.7(6) . 5_566
O1 Ta1 O2 104.5(6) 6_565 5_566
O1 Ta1 O2 70.3(6) 5_566 5_566
O2 Ta1 O2 156.0(8) 6_565 5_566
O2 Ta1 O2 180.000(1) . 5_566
O2 Ta1 O2 24.0(8) 2_556 5_566
O1 O1 O3 149.2(13) 6_565 .
O1 O1 C2 136.4(7) 6_565 .
O3 O1 C2 73.3(15) . .
O1 O1 O3 15.5(7) 6_565 6_565
O3 O1 O3 133.7(19) . 6_565
C2 O1 O3 150.7(12) . 6_565
O1 O1 O4 134.8(7) 6_565 .
O3 O1 O4 14.3(11) . .
C2 O1 O4 87.1(11) . .
O3 O1 O4 119.3(11) 6_565 .
O1 O1 C14 77.0(4) 6_565 .
O3 O1 C14 133.7(16) . .
C2 O1 C14 63.4(7) . .
O3 O1 C14 92.4(8) 6_565 .
O4 O1 C14 147.9(10) . .
O1 O1 Ta1 77.8(4) 6_565 .
O3 O1 Ta1 77.6(13) . .
C2 O1 Ta1 121.5(10) . .
O3 O1 Ta1 65.8(8) 6_565 .
O4 O1 Ta1 66.1(7) . .
C14 O1 Ta1 139.4(9) . .
O1 O1 Na1 80.6(3) 6_565 .
O3 O1 Na1 79.2(15) . .
C2 O1 Na1 134.7(9) . .
O3 O1 Na1 70.9(7) 6_565 .
O4 O1 Na1 70.8(7) . .
C14 O1 Na1 120.7(9) . .
Ta1 O1 Na1 85.5(5) . .
O2 O2 O5 150.0(13) 6_565 .
O2 O2 C1 136.1(7) 6_565 .
O5 O2 C1 72.5(14) . .
O2 O2 O5 15.2(6) 6_565 6_565
O5 O2 O5 134.8(18) . 6_565
C1 O2 O5 149.9(11) . 6_565
O2 O2 O6 135.1(7) 6_565 .
O5 O2 O6 14.9(11) . .
C1 O2 O6 86.9(10) . .
O5 O2 O6 119.9(11) 6_565 .
O2 O2 C13 77.2(4) 6_565 .
O5 O2 C13 132.7(15) . .
C1 O2 C13 62.9(7) . .
O5 O2 C13 92.4(7) 6_565 .
O6 O2 C13 147.5(10) . .
O2 O2 Ta1 78.0(4) 6_565 .
O5 O2 Ta1 78.0(13) . .
C1 O2 Ta1 120.5(9) . .
O5 O2 Ta1 66.1(7) 6_565 .
O6 O2 Ta1 66.1(7) . .
C13 O2 Ta1 138.5(9) . .
O2 O2 Na1 80.6(3) 6_565 5_566
O5 O2 Na1 80.0(13) . 5_566
C1 O2 Na1 135.4(9) . 5_566
O5 O2 Na1 71.2(7) 6_565 5_566
O6 O2 Na1 71.1(7) . 5_566
C13 O2 Na1 121.8(9) . 5_566
Ta1 O2 Na1 85.9(5) . 5_566
O4 O3 O1 151(2) . .
O4 O3 C2 136(2) . .
O1 O3 C2 72.1(14) . .
O4 O3 O1 135.5(18) . 6_565
O1 O3 O1 15.3(8) . 6_565
C2 O3 O1 87.0(10) . 6_565
O4 O3 O6 15.0(12) . 2_556
O1 O3 O6 135.9(17) . 2_556
C2 O3 O6 149.3(16) . 2_556
O1 O3 O6 120.5(12) 6_565 2_556
O4 O3 C12 77.4(17) . .
O1 O3 C12 131.7(17) . .
C2 O3 C12 62.0(8) . .
O1 O3 C12 147.0(11) 6_565 .
O6 O3 C12 92.4(12) 2_556 .
O4 O3 Ta1 78.3(14) . .
O1 O3 Ta1 77.7(13) . .
C2 O3 Ta1 121.0(9) . .
O1 O3 Ta1 65.8(7) 6_565 .
O6 O3 Ta1 66.6(7) 2_556 .
C12 O3 Ta1 138.7(12) . .
O4 O3 Na1 80.3(14) . .
O1 O3 Na1 81.8(16) . .
C2 O3 Na1 135.6(12) . .
O1 O3 Na1 72.2(9) 6_565 .
O6 O3 Na1 71.1(7) 2_556 .
C12 O3 Na1 121.6(7) . .
Ta1 O3 Na1 86.1(5) . .
O3 O4 O6 151(2) . 2_556
O3 O4 C3 135(2) . 2_556
O6 O4 C3 72.6(17) 2_556 2_556
O3 O4 O5 135.5(18) . 2_556
O6 O4 O5 15.0(11) 2_556 2_556
C3 O4 O5 86.9(13) 2_556 2_556
O3 O4 O1 14.8(12) . .
O6 O4 O1 135.8(17) 2_556 .
C3 O4 O1 148.6(13) 2_556 .
O5 O4 O1 120.8(11) 2_556 .
O3 O4 C12 77.3(17) . .
O6 O4 C12 132.1(18) 2_556 .
C3 O4 C12 62.4(8) 2_556 .
O5 O4 C12 147.1(13) 2_556 .
O1 O4 C12 92.1(11) . .
O3 O4 Ta1 77.8(13) . .
O6 O4 Ta1 78.5(14) 2_556 .
C3 O4 Ta1 120.6(12) 2_556 .
O5 O4 Ta1 66.4(8) 2_556 .
O1 O4 Ta1 65.9(7) . .
C12 O4 Ta1 138.4(9) . .
O3 O4 Na1 81.2(16) . .
O6 O4 Na1 80.0(13) 2_556 .
C3 O4 Na1 135.5(10) 2_556 .
O5 O4 Na1 71.3(7) 2_556 .
O1 O4 Na1 72.5(8) . .
C12 O4 Na1 121.9(9) . .
Ta1 O4 Na1 86.2(5) . .
O6 O5 O2 150(2) . .
O6 O5 C1 136.1(19) . .
O2 O5 C1 72.5(14) . .
O6 O5 O2 135.0(17) . 6_565
O2 O5 O2 14.8(8) . 6_565
C1 O5 O2 86.8(10) . 6_565
O6 O5 O4 15.4(12) . 2_556
O2 O5 O4 134.4(17) . 2_556
C1 O5 O4 149.7(14) . 2_556
O2 O5 O4 119.6(11) 6_565 2_556
O6 O5 C11 77.8(16) . .
O2 O5 C11 132.4(16) . .
C1 O5 C11 62.4(8) . .
O2 O5 C11 147.1(11) 6_565 .
O4 O5 C11 93.2(11) 2_556 .
O6 O5 Ta1 78.0(13) . .
O2 O5 Ta1 77.4(14) . .
C1 O5 Ta1 120.2(10) . .
O2 O5 Ta1 65.8(8) 6_565 .
O4 O5 Ta1 65.5(7) 2_556 .
C11 O5 Ta1 138.6(9) . .
O6 O5 Na1 80.4(13) . 5_566
O2 O5 Na1 80.7(13) . 5_566
C1 O5 Na1 135.8(10) . 5_566
O2 O5 Na1 71.5(7) 6_565 5_566
O4 O5 Na1 71.5(8) 2_556 5_566
C11 O5 Na1 122.1(8) . 5_566
Ta1 O5 Na1 85.9(5) . 5_566
O5 O6 O4 150(2) . 2_556
O5 O6 C3 135.7(19) . .
O4 O6 C3 72.8(16) 2_556 .
O5 O6 O2 15.3(12) . .
O4 O6 O2 134.3(17) 2_556 .
C3 O6 O2 149.3(14) . .
O5 O6 O3 135.1(17) . 2_556
O4 O6 O3 14.5(12) 2_556 2_556
C3 O6 O3 86.8(13) . 2_556
O2 O6 O3 119.8(11) . 2_556
O5 O6 C11 76.5(16) . .
O4 O6 C11 133.9(18) 2_556 .
C3 O6 C11 63.5(8) . .
O2 O6 C11 91.8(11) . .
O3 O6 C11 148.3(13) 2_556 .
O5 O6 Ta1 78.0(14) . .
O4 O6 Ta1 76.8(13) 2_556 .
C3 O6 Ta1 119.8(9) . .
O2 O6 Ta1 65.8(7) . .
O3 O6 Ta1 65.5(7) 2_556 .
C11 O6 Ta1 137.9(10) . .
O5 O6 Na1 80.8(13) . 5_566
O4 O6 Na1 80.7(14) 2_556 5_566
C3 O6 Na1 136.0(10) . 5_566
O2 O6 Na1 71.6(7) . 5_566
O3 O6 Na1 71.9(8) 2_556 5_566
C11 O6 Na1 121.8(8) . 5_566
Ta1 O6 Na1 86.0(5) . 5_566
O5 C1 O2 35.0(7) . .
O5 C1 C23 112.2(13) . .
O2 C1 C23 135.5(13) . .
O5 C1 C22 135.5(13) . .
O2 C1 C22 112.3(14) . .
C23 C1 C22 67.8(17) . .
O5 C1 C2 105.3(9) . .
O2 C1 C2 105.1(9) . .
C23 C1 C2 115.0(13) . .
C22 C1 C2 114.8(12) . .
O5 C1 C11 71.2(9) . .
O2 C1 C11 104.9(9) . .
C23 C1 C11 47.6(12) . .
C22 C1 C11 113.7(13) . .
C2 C1 C11 105.1(8) . .
O5 C1 C13 104.8(10) . .
O2 C1 C13 71.2(9) . .
C23 C1 C13 113.4(13) . .
C22 C1 C13 47.4(12) . .
C2 C1 C13 105.2(9) . .
C11 C1 C13 149.3(9) . .
O1 C2 O3 34.6(8) . .
O1 C2 C25 135.8(13) . .
O3 C2 C25 112.4(14) . .
O1 C2 C21 112.1(14) . .
O3 C2 C21 135.3(14) . .
C25 C2 C21 68.6(17) . .
O1 C2 C1 104.2(9) . .
O3 C2 C1 104.8(9) . .
C25 C2 C1 115.5(12) . .
C21 C2 C1 114.7(12) . .
O1 C2 C12 105.2(9) . .
O3 C2 C12 71.7(9) . .
C25 C2 C12 47.2(13) . .
C21 C2 C12 114.2(14) . .
C1 C2 C12 105.4(8) . .
O1 C2 C14 70.5(9) . .
O3 C2 C14 103.8(11) . .
C25 C2 C14 114.1(13) . .
C21 C2 C14 47.4(13) . .
C1 C2 C14 105.1(9) . .
C12 C2 C14 149.2(9) . .
O4 C3 O6 34.6(8) 2_556 .
O4 C3 C26 113.2(14) 2_556 2_556
O6 C3 C26 135.6(13) . 2_556
O4 C3 C24 135.0(13) 2_556 .
O6 C3 C24 111.5(14) . .
C26 C3 C24 67.5(17) 2_556 .
O4 C3 C3 105.1(7) 2_556 2_556
O6 C3 C3 105.4(7) . 2_556
C26 C3 C3 115.1(12) 2_556 2_556
C24 C3 C3 115.0(12) . 2_556
O4 C3 C12 71.3(10) 2_556 2_556
O6 C3 C12 104.6(10) . 2_556
C26 C3 C12 48.4(13) 2_556 2_556
C24 C3 C12 114.0(13) . 2_556
C3 C3 C12 105.5(10) 2_556 2_556
O4 C3 C11 103.9(10) 2_556 .
O6 C3 C11 70.4(9) . .
C26 C3 C11 113.6(14) 2_556 .
C24 C3 C11 47.7(12) . .
C3 C3 C11 104.8(9) 2_556 .
C12 C3 C11 149.5(8) 2_556 .
C23 C11 C24 136.0(18) . .
C23 C11 C1 57.4(13) . .
C24 C11 C1 166.3(14) . .
C23 C11 C3 167.0(15) . .
C24 C11 C3 56.6(12) . .
C1 C11 C3 109.9(7) . .
C23 C11 O6 124.0(16) . .
C24 C11 O6 97.5(14) . .
C1 C11 O6 71.1(8) . .
C3 C11 O6 46.1(7) . .
C23 C11 O5 98.5(15) . .
C24 C11 O5 123.0(15) . .
C1 C11 O5 46.4(7) . .
C3 C11 O5 70.8(7) . .
O6 C11 O5 25.7(6) . .
C25 C12 C26 136.3(18) . .
C25 C12 C2 57.4(13) . .
C26 C12 C2 166.0(14) . .
C25 C12 C3 167.1(15) . 2_556
C26 C12 C3 56.4(12) . 2_556
C2 C12 C3 109.8(7) . 2_556
C25 C12 O3 98.4(16) . .
C26 C12 O3 122.8(15) . .
C2 C12 O3 46.3(7) . .
C3 C12 O3 70.6(8) 2_556 .
C25 C12 O4 123.5(16) . .
C26 C12 O4 97.6(15) . .
C2 C12 O4 70.6(8) . .
C3 C12 O4 46.3(8) 2_556 .
O3 C12 O4 25.3(6) . .
C22 C13 C22 137(2) . 6_565
C22 C13 C1 56.6(11) . .
C22 C13 C1 166.0(15) 6_565 .
C22 C13 C1 166.0(15) . 6_565
C22 C13 C1 56.6(11) 6_565 6_565
C1 C13 C1 109.5(10) . 6_565
C22 C13 O2 97.6(13) . .
C22 C13 O2 122.9(14) 6_565 .
C1 C13 O2 45.9(6) . .
C1 C13 O2 70.5(7) 6_565 .
C22 C13 O2 122.9(14) . 6_565
C22 C13 O2 97.6(13) 6_565 6_565
C1 C13 O2 70.5(7) . 6_565
C1 C13 O2 45.9(6) 6_565 6_565
O2 C13 O2 25.6(8) . 6_565
C21 C14 C21 134(2) 6_565 .
C21 C14 C2 167.4(14) 6_565 .
C21 C14 C2 57.6(11) . .
C21 C14 C2 57.6(11) 6_565 6_565
C21 C14 C2 167.4(14) . 6_565
C2 C14 C2 110.3(10) . 6_565
C21 C14 O1 124.8(14) 6_565 .
C21 C14 O1 98.9(13) . .
C2 C14 O1 46.1(6) . .
C2 C14 O1 71.1(7) 6_565 .
C21 C14 O1 98.9(13) 6_565 6_565
C21 C14 O1 124.8(14) . 6_565
C2 C14 O1 71.1(7) . 6_565
C2 C14 O1 46.1(6) 6_565 6_565
O1 C14 O1 26.1(9) . 6_565
C14 C21 C2 75.0(12) . .
C14 C21 C25 127.5(17) . .
C2 C21 C25 55.1(12) . .
C13 C22 C1 76.0(13) . .
C13 C22 C23 129.6(17) . .
C1 C22 C23 56.1(13) . .
C11 C23 C1 75.1(13) . .
C11 C23 C22 128.8(19) . .
C1 C23 C22 56.1(13) . .
C11 C24 C3 75.6(13) . .
C11 C24 C26 129.1(18) . 2_556
C3 C24 C26 55.7(12) . 2_556
C12 C25 C2 75.4(13) . .
C12 C25 C21 129.4(19) . .
C2 C25 C21 56.3(13) . .
C12 C26 C3 75.2(13) . 2_556
C12 C26 C24 129.4(19) . 2_556
C3 C26 C24 56.8(13) 2_556 2_556
O1A Na1 O2A 52.0(6) . 2
O1A Na1 O2A 52.0(6) . 5_565
O2A Na1 O2A 98.4(10) 2 5_565
O1A Na1 O2A 96.6(7) . .
O2A Na1 O2A 50.2(11) 2 .
O2A Na1 O2A 119.8(4) 5_565 .
O1A Na1 O2A 96.6(7) . 6_565
O2A Na1 O2A 119.8(4) 2 6_565
O2A Na1 O2A 50.2(11) 5_565 6_565
O2A Na1 O2A 97.4(11) . 6_565
O1A Na1 O1A 120.1(5) . 5_565
O2A Na1 O1A 96.8(6) 2 5_565
O2A Na1 O1A 96.8(6) 5_565 5_565
O2A Na1 O1A 51.7(6) . 5_565
O2A Na1 O1A 51.7(6) 6_565 5_565
O1A Na1 Na1 60.3(5) . 5_565
O2A Na1 Na1 60.3(4) 2 5_565
O2A Na1 Na1 60.3(4) 5_565 5_565
O2A Na1 Na1 59.5(6) . 5_565
O2A Na1 Na1 59.5(6) 6_565 5_565
O1A Na1 Na1 59.8(4) 5_565 5_565
O1A Na1 O4 103.9(6) . .
O2A Na1 O4 140.9(7) 2 .
O2A Na1 O4 81.4(5) 5_565 .
O2A Na1 O4 157.2(7) . .
O2A Na1 O4 90.2(6) 6_565 .
O1A Na1 O4 122.1(6) 5_565 .
Na1 Na1 O4 140.7(3) 5_565 .
O1A Na1 O4 103.9(6) . 6_565
O2A Na1 O4 81.4(5) 2 6_565
O2A Na1 O4 140.9(7) 5_565 6_565
O2A Na1 O4 90.2(6) . 6_565
O2A Na1 O4 157.2(7) 6_565 6_565
O1A Na1 O4 122.1(6) 5_565 6_565
Na1 Na1 O4 140.7(3) 5_565 6_565
O4 Na1 O4 75.4(6) . 6_565
O1A Na1 O6 121.9(6) . 2_556
O2A Na1 O6 156.9(6) 2 2_556
O2A Na1 O6 89.2(6) 5_565 2_556
O2A Na1 O6 141.4(8) . 2_556
O2A Na1 O6 81.7(6) 6_565 2_556
O1A Na1 O6 103.9(5) 5_565 2_556
Na1 Na1 O6 140.3(3) 5_565 2_556
O4 Na1 O6 19.3(4) . 2_556
O4 Na1 O6 79.1(5) 6_565 2_556
O1A Na1 O6 121.9(6) . 5_566
O2A Na1 O6 89.2(6) 2 5_566
O2A Na1 O6 156.9(6) 5_565 5_566
O2A Na1 O6 81.7(6) . 5_566
O2A Na1 O6 141.4(8) 6_565 5_566
O1A Na1 O6 103.9(5) 5_565 5_566
Na1 Na1 O6 140.3(3) 5_565 5_566
O4 Na1 O6 79.1(5) . 5_566
O4 Na1 O6 19.3(4) 6_565 5_566
O6 Na1 O6 76.1(7) 2_556 5_566
O1A Na1 O5 140.6(5) . 2_556
O2A Na1 O5 156.4(6) 2 2_556
O2A Na1 O5 103.3(6) 5_565 2_556
O2A Na1 O5 122.6(7) . 2_556
O2A Na1 O5 81.8(6) 6_565 2_556
O1A Na1 O5 89.7(5) 5_565 2_556
Na1 Na1 O5 140.2(5) 5_565 2_556
O4 Na1 O5 37.2(5) . 2_556
O4 Na1 O5 76.0(5) 6_565 2_556
O6 Na1 O5 18.8(4) 2_556 2_556
O6 Na1 O5 67.2(6) 5_566 2_556
C2A O1A C2A 80(3) 6_565 .
C2A O1A Na1 131.4(14) 6_565 .
C2A O1A Na1 131.4(14) . .
C2A O1A Na1 131.5(15) 6_565 5_565
C2A O1A Na1 131.5(15) . 5_565
Na1 O1A Na1 59.9(5) . 5_565
C3A O2A C1A 81(2) 5_565 .
C3A O2A Na1 130(2) 5_565 5_565
C1A O2A Na1 133.0(18) . 5_565
C3A O2A Na1 132(2) 5_565 .
C1A O2A Na1 129.9(18) . .
Na1 O2A Na1 60.2(4) 5_565 .
C1A C1A O2A 100.5(14) 2 .
C3A C2A O1A 99(2) . .
C2A C3A O2A 101(3) . 5_565
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Ta1 O3 1.957(13) 2_556
Ta1 O3 1.957(13) 6_565
Ta1 O3 1.957(13) 5_566
Ta1 O3 1.957(13) .
Ta1 O1 1.958(12) 2_556
Ta1 O1 1.958(12) .
Ta1 O1 1.958(12) 6_565
Ta1 O1 1.958(12) 5_566
Ta1 O2 1.969(13) 6_565
Ta1 O2 1.969(13) .
Ta1 O2 1.969(13) 2_556
Ta1 O2 1.969(13) 5_566
O1 O1 0.83(3) 6_565
O1 O3 0.836(19) .
O1 C2 1.400(16) .
O1 O3 1.60(3) 6_565
O1 O4 1.59(2) .
O1 C14 1.83(2) .
O1 Na1 2.540(16) .
O2 O2 0.82(3) 6_565
O2 O5 0.843(17) .
O2 C1 1.404(15) .
O2 O5 1.61(2) 6_565
O2 O6 1.60(2) .
O2 C13 1.85(2) .
O2 Na1 2.517(14) 5_566
O3 O4 0.812(19) .
O3 C2 1.409(17) .
O3 O1 1.60(3) 6_565
O3 O6 1.60(2) 2_556
O3 C12 1.85(2) .
O3 Na1 2.521(16) .
O4 O6 0.841(19) 2_556
O4 C3 1.414(19) 2_556
O4 O5 1.60(2) 2_556
O4 C12 1.85(2) .
O4 Na1 2.515(16) .
O5 O6 0.819(18) .
O5 C1 1.404(17) .
O5 O2 1.61(2) 6_565
O5 O4 1.60(2) 2_556
O5 C11 1.835(19) .
O5 Na1 2.513(13) 5_566
O6 O4 0.841(19) 2_556
O6 C3 1.412(17) .
O6 O3 1.60(2) 2_556
O6 C11 1.845(19) .
O6 Na1 2.509(14) 5_566
C1 C23 1.50(3) .
C1 C22 1.50(2) .
C1 C2 1.552(13) .
C1 C11 1.719(17) .
C1 C13 1.740(14) .
C2 C25 1.50(2) .
C2 C21 1.52(2) .
C2 C12 1.721(18) .
C2 C14 1.739(14) .
C3 O4 1.414(19) 2_556
C3 C26 1.49(2) 2_556
C3 C24 1.51(2) .
C3 C3 1.549(17) 2_556
C3 C12 1.732(17) 2_556
C3 C11 1.752(16) .
C11 C23 1.31(3) .
C11 C24 1.34(3) .
C12 C25 1.31(3) .
C12 C26 1.34(3) .
C12 C3 1.732(17) 2_556
C13 C22 1.32(3) .
C13 C22 1.32(3) 6_565
C13 C1 1.740(14) 6_565
C13 O2 1.85(2) 6_565
C14 C21 1.33(3) 6_565
C14 C21 1.33(3) .
C14 C2 1.739(14) 6_565
C14 O1 1.83(2) 6_565
C21 C25 1.70(5) .
C22 C23 1.67(4) .
C24 C26 1.67(4) 2_556
C26 C3 1.49(2) 2_556
C26 C24 1.67(4) 2_556
Na1 O1A 2.236(16) .
Na1 O2A 2.222(19) 2
Na1 O2A 2.222(19) 5_565
Na1 O2A 2.239(12) .
Na1 O2A 2.239(12) 6_565
Na1 O1A 2.245(19) 5_565
Na1 Na1 2.237(10) 5_565
Na1 O4 2.515(16) 6_565
Na1 O6 2.509(14) 2_556
Na1 O6 2.509(14) 5_566
Na1 O5 2.513(13) 2_556
O1A C2A 1.70(3) 6_565
O1A C2A 1.70(3) .
O1A Na1 2.245(19) 5_565
O2A C3A 1.69(4) 5_565
O2A C1A 1.62(4) .
O2A Na1 2.222(19) 5_565
C1A C1A 1.30(6) 2
C2A C3A 1.36(5) .
C3A O2A 1.69(4) 5_565
